Review Article | Open Access
Resin-Dentin Bonding Interface: Mechanisms of Degradation and Strategies for Stabilization of the Hybrid Layer
Several studies have shown that the dentin-resin interface is unstable due to poor infiltration of resin monomers into the demineralized dentin matrix. This phenomenon is related to the incomplete infiltration of the adhesive system into the network of exposed collagen fibrils, mainly due to the difficulty of displacement and subsequent replacement of trapped water between interfibrillar spaces, avoiding adequate hybridization within the network of collagen fibrils. Thus, unprotected fibrils are exposed to undergo denaturation and are susceptible to cyclic fatigue rupture after being subjected to repetitive loads during function. The aqueous inclusions within the hybrid layer serve as a functional medium for the hydrolysis of the resin matrix, giving rise to the activity of esterases and collagenolytic enzymes, such as matrix metalloproteinases, which play a fundamental role in the degradation process of the hybrid layer. Achieving better interdiffusion of the adhesive system in the network of collagen fibrils and the substrate stability in the hybrid layer through different strategies are key events for the interfacial microstructure to adequately function. Hence, it is important to review the factors related to the mechanisms of degradation and stabilization of the hybrid layer to support the implementation of new materials and techniques in the future. The enzymatic degradation of collagen matrix, together with resin leaching, has led to seeking strategies that inhibit the endogenous proteases, cross-linking the denudated collagen fibrils and improving the adhesive penetration removing water from the interface. Some of dentin treatments have yielded promising results and require more research to be validated. A longer durability of adhesive restorations could resolve a variety of clinical problems, such as microleakage, recurrent caries, postoperative sensitivity, and restoration integrity.
Composite resin is a restorative material widely used in dentistry for filling dental cavities and cementing indirect restorations and aesthetic restorations [1, 2]. The resin-dentin bond depends on the infiltration of the adhesive system into the collagen matrix of the dentin, which is exposed through acid conditioning. The resin-dentin interdiffusion zone, called the “hybrid layer,” fulfills a fundamental function in the micromechanical retention of the restoration . It has been established that the infiltration of collagen by the adhesive is incomplete since its penetration capacity is lower than the depth of conditioning of the etching agent. Additionally, removing residual water in the dentin matrix is difficult [4, 5]. Both of these are reasons why a portion of collagen remains unprotected, which results in the activation of endogenous proteases, called extracellular matrix metalloproteinases (MMPs) and cysteine cathepsins (CTs), present in dentin. As collagenolytic enzymes, MMPs and CTs hydrolyze the organic matrix of demineralized dentin, an event that triggers hybrid layer degradation [6, 7].
To counteract the effect of MMPs, the use of nonspecific synthetic inhibitors, such as chlorhexidine (CHX) [8, 9], has been suggested. However, it has been shown to be effective only in short and medium terms due its binding to dentin being electrostatic in nature . As a result, its inhibitory capacity decreases in less than 2 years . On the other hand, Breschi et al.  reported the effectiveness of 0,2% CHX to inhibit MMPs activity in acid-etched adhesive-infiltrated dentin aged for 2 years. Recently, the experimental use of cross-linking agents of collagen has been proposed as a strategy. This technique promotes resistance to enzymatic degradation and has the ability to inhibit the activity of MMPs. Flavonoid-type polyphenolic compounds, such as proanthocyanidins, quercetin, and curcumin, have chemical structures that favor their function as cross-linking agents. However, their benefits in clinically relevant protocols have not been shown since the application times required and their depth of penetration do not make them effective within clinical protocols [13–15].
This hydrolytic degradation of the adhesive interface generates adverse clinical consequences, such as dentin hypersensitivity, marginal pigmentation, and possible secondary caries, thus decreasing the longevity of the restorations . Such events result in high biological and economic costs associated with the need to replace restorations .
The objective of this study was to review the literature to identify factors that influence degradation of the resin-dentin adhesive interface and strategies that have been proposed to stabilize the hybrid layer and improve the durability of adhesive restorations.
An electronic search was carried out to identify relevant manuscripts in the following databases: PubMed, Scielo, Cochrane, Elsevier, EBSCO, LILACS, and Web of Science, using terms selected according to the Medical Subject Headings (MeSH): bonding, collagen, cross-linking reagents, matrix metalloproteinases, dentin, dentin bonding agents, endopeptidases, cysteine cathepsins. The reference lists of the included articles were also reviewed. There was no restriction of year or language for the publications, and the last search was conducted in Nov 2018. This review aimed to collect the most outstanding information that described the mechanisms that occur during degradation processes of resin adhesives and collagen matrix, as well as some of the experimental strategies to stabilize the resin-dentin interface, mainly related to inhibition of MMPs and collagen cross-linking.
2.1. Dentin as a Substrate for Adhesion
Dentin, a biological, complex, and dynamic tissue, underlies the dental enamel and is related histologically, embryologically, and functionally to the dental pulp. Odontoblasts are highly specialized cells that produce both collagen and noncollagen proteins to build the dentinal extracellular matrix . Dentin is composed of 47% (vol) apatite crystals, 20% (vol) water, and 33% (vol) organic material. Dentin has a tubular structure in a radial arrangement, where tubules run from the pulp to the dentinoenamel junction (DEJ) surrounded by intertubular dentin. Close to the pulp, the tubule number is 45,000-65,000/mm2 and reaches 22% of the dentinal area, while in outer dentin it is 15,000-20,000/mm2 representing 1% of the dentinal area. In the same way, the diameter of the tubules close to the pulp is larger (3-4 μm) and smaller near the DEJ (1,7 μm) . The regional differences in the intertubular area and tubule orientation may influence the efficacy of the dentinal adhesives .
Type I collagen makes up 90% of the organic material, with noncollagenous proteins accounting for the remainder [18, 20]. These proportions vary according to the region of the tooth and are affected by physiological processes, such as aging, and pathological processes, such as dental caries . Dentin conditioning by acid etching also alters the composition of dentin, whereby the amount of water present changes from 18% to 50-70% by volume, with great implications on the physical characteristics of the tissue .
Collagen is a protein composed of a sequence of amino acids: glycine, lysine, proline, and their hydroxylated products, mainly hydroxyproline and hydroxylysine. It is synthesized from a larger molecule, tropocollagen, which is cleaved at the level of terminal carboxyl and amino groups with a periodicity of 67-69 nm, which in turn facilitates cross-linking. The intrinsic cross-linking ability of collagen is enhanced by enzymatic and nonenzymatic reactions. Enzymatic reactions form lysine-lysine covalent bonds, which are mediated by the hydroxylation of lysine, glycosylation, and molecular turnover rate. Nonenzymatic cross-linking involves oxidation and glycation processes [23, 24].
The quaternary structure of collagen has a triple helix with an arrangement that makes it very stable and resistant to degradation. Collagen plays a prominent role in the tensile strength, the elastic modulus and biochemical properties of dentin, which depend on its degree of cross-linking  (Figure 1).
Noncollagenous proteins, such as proteoglycans (PG) (e.g., chondroitin-4/6-sulfate, decorin, biglycan, lumican, and fibromodulin) [26, 27], and small integrin-binding ligand N-linked glycoproteins (SIBLING), such as bone sialoprotein, osteopontin, protein dentinal-1 matrix, and dentin sialophosphoprotein, play important roles in dentinogenesis, including regulation functions and control of crystal growth, fibrillogenesis, and mineralization  (Figure 2).
2.2. MMPs: Structure and Function
MMPs are a family of enzymes and 23 types have been described in humans. They are dependent on calcium and zinc for activity and are characterized by having four domains in their composition: the peptide-signal domain, the propeptide domain (composed of cysteine with its sulfhydryl groups), a catalytic domain (with zinc at the site of catalytic activity together with histidine and calcium residues), and a hemopexin-type domain that serves to bind to the substrate and which is the site where specific tissue inhibitors bind  (Figure 3).
These enzymes are produced by leukocytes and fibroblast-like cells capable of synthesizing extracellular mineralized matrix, including the cells of the dental pulp. They are secreted in the form of proenzyme (inactive enzyme), remaining as zymogens until activated. The proenzyme is characterized by binding to the sulfhydryl groups present in the cysteine component of the propeptide domain, with zinc, although present in the catalytic domain, being unavailable for catalytic activity. The process of activation of the enzyme is initiated by the breakdown of the zinc-cysteine interaction, which is called the cysteine switch. This process is key to understanding the functioning of these enzymes and their possible inhibition [31–34].
During tooth development, close ectomesenchymal communication is required, and MMPs play an important role in this interaction. In early stages of odontogenesis, this interaction determines dental morphogenesis and in late stages, determines the differentiation of odontoblasts and ameloblasts [35, 36]. Mesenchymal cells express, at least, MMP-1, MMP-2, MMP-3, MMP-8, MMP-9, MMP-14, and MMP-20. Additionally, the role of MMPs in the process of reabsorption of extracellular matrix proteins has been proposed as a regulatory mechanism necessary for correct mineralization of the dental structure . Some in the form of proenzymes are trapped inside the mineralized dentin matrix during dentinal development , and because of their collagenolytic protease activity, they can hydrolyze the components of the extracellular matrix when activated by physical or chemical stimuli . These proteases play a central role in several physiological processes, such as development, tissue remodeling, and angiogenesis .
MMPs are involved in different pathological processes, such as periodontal disease and dental caries. Recent studies have revealed their role in the breakdown of the collagen matrix in the pathogenesis of caries [33, 41], with potential and relevant implications for dentin binding . In addition, they may be present in saliva , peritubular dentin, and presumably, dentinal fluid .
Of the proposed classifications to name MMPs, the one most used was established based on the substrate on which they have activity. Therefore, they are named as collagenases (MMP-1, MMP-8, MMP-13, and MMP-18), gelatinases (MMP-2 and MMP-9), stromelysins (MMP-3 and MMP-10), matrilysins (MMP-7 and MMP-26), and membrane-type MMP (MMP-14, MMP-15, MMP-16, and MMP-24) (Bali et al., 2016). MMPs found in human dentin are MMP-2, MMP-9 , MMP-8 , MMP-3  and MMP-20 .
2.3. Degradation of the Adhesive Interface
Composite resins, as restorative materials, base their retention on an adhesive process that unites them to the dental structure. Adhesion to dentin is a clinical challenge, because it is a tissue of heterogeneous composition, with high organic content and the presence of moisture [2, 22]. The adhesion of resinous systems to the dentin requires the infiltration of collagen fibrils that have been exposed by previous acid conditioning, with the resin monomers present in the adhesive generating a resin-dentin interdiffusion zone, called the hybrid layer . This is necessary for the micromechanical retention of the restoration.
It is widely accepted that after the use of current dental adhesives, a degradation of the dentin-resin adhesive interface occurs . Among the factors that intervene with the degradation of the adhesive interface, the following have been proposed:
2.3.1. Degradation of the Adhesive Resin
The use of hydrophilic monomers in adhesive systems, such as 2-hydroxyethyl methacrylate (HEMA), seeks to improve infiltration of the exposed collagen network, which is inherently humid. This has been reported to result in an immediate improvement of bond strength ; but the longevity of this dentin-resin bond is compromised with the use of these adhesive systems [48–50].
The presence of water in the adhesive interface generates a weak hybrid layer, in which the phenomena of hydrolysis and leaching of resin adhesives occur [16, 51]. Current adhesives include in their formulation hydrophilic and hydrophobic components that, in aqueous solution, produce nanophase separation of adhesives . The hydrophilic elements penetrate the interior of the hybrid layer, while the hydrophobic monomers remain on the surface. Being hydrophobic, the camphorquinones do not penetrate, leading to inadequate polymerization in the deepest zone of the hybrid layer .
The incomplete polymerization of the hydrophilic portion of the adhesives and the aqueous sorption of the material allow the mobilization of water, which forms large aqueous channels within the hybrid layer  (Figure 4.). Additionally, the action of esterase enzymes that come from saliva, pulp, and bacteria  break the ester bonds present in the HEMA, which generates hydrophilic cytotoxic by-products such as ethylene glycol, as well as hydrophobic ones such as methacrylic acid .
This phenomenon can be triggered not only with etch-and-rinse (E&R) adhesives but also with self-etching (SE) adhesives [31, 57]. Several studies, such as those by Nishitani et al.  and Mazonni et al. , have established that the monomeric systems incorporated in self-etching adhesives are also susceptible to hydrolytic degradation and allow collagenolytic and gelatinolytic activities within the collagen matrix due to their low pH.
2.3.2. Incomplete Infiltration of the Adhesive in the Exposed Collagen Network
In the E&R technique, the difference between penetration of the adhesive and action of the conditioning acid agent leads to an incomplete hybridization of the exposed collagen network. As such, a portion of the collagen fibrils remain uninfused, being more susceptible to hydrolytic degradation, which leads to nanopercolation  (Figure 5).
The inability of resin monomers to replace both free and collagen-bound water present in the inter- and intrafibrillar compartments is a limitation to achieve a complete and stable hybrid layer [59, 60].
Additionally, highly hydrated proteoglycan hydrogels are found in interfibrillary spaces . These act as filters that trap the monomers of large molecules, such as BisGMA, and only allow the passage of small monomers, such as HEMA, toward the base of the hybrid layer. HEMA produces weak linear chains that, when subjected to stresses, lead to failure due to cyclic fatigue of the collagen chains .
2.3.3. Degradation of Collagen by Endopeptidases
Pashley et al.  were the first to demonstrate the degradation of collagen fibrils in the absence of bacteria, suggesting proteolytic activity within the dentin. Dentin contains a large amount of MMPs in inactive form, which are trapped in the tissue, from the mineralization process and can be activated by different chemical and physical mechanisms. The incomplete infiltration of the collagen network by resin monomers makes it especially vulnerable to hydrolytic degradation mainly by MMPs . These enzymes have a great capacity to degrade almost all components of the extracellular matrix, acting in a synchronous manner, so that some MMPs require previous activation of other proteases. This is how, for example, MMP-8 has the ability to degrade collagen, resulting in the release of 3/4- to 1/4- length peptides, denaturing the triple-helical structure, allowing the subsequent activity of gelatinases (MMP-2 and MMP-9) to digest peptide residues .
MMPs can be activated in vivo by proteases and other MMPs, in vitro by chemical agents such as modifiers of the sulfhydryl groups, chaotropic agents, and reactive oxygen, as well as physical agents such as low pH and heat [30, 34, 39].
The degradation of collagen fibrils in vivo has been directly correlated with the activation of MMPs induced by the application of dentinal adhesive systems [11, 63, 64]. Initially, the acid conditioning procedure was believed to favor the release and activation of proenzymes trapped inside the mineralized dentin , which induces a collagenolytic activity within the hybridized dentin. However, some authors have reported that the very low pH (0.7-1) of phosphoric acid in the conditioning can denature MMPs by preventing their action [5–7]. In contrast, when mixing powder of demineralized dentin with SE adhesives it has been shown that the pH, initially very low, rises to neutrality quickly, and the SEM revealed the presence of a dense insoluble precipitate that is deposited on the surface of the conditioned collagen fibrils, which could temporarily prevent the activity of MMPs . Sabatini & Pashley  propose that acid phosphate groups bind with Ca2+ and become deposited on the surface of the dentin.
The action of MMP-2 and MMP-9 has been confirmed by means of specific tests for different types of dentinal adhesives. Lehmann et al.  reported that the application of the adhesive increases the synthesis of MMP-2 in human odontoblasts, which possibly increases its action by migration through the dentinal tubules to the hybrid layer. With regard to SE adhesives, Mazzoni et al.  reported that there is evidence that partially demineralized dentin activity was found in MMP-2 and MMP-9 in human dentin. This effect is attributed to the low pH which triggers the cysteine switch and activates latent forms of the enzymes to exert their effect on the catalytic domain. It also decreases the inhibitory activity of tissue inhibitors of MMP.
CTs are host-derived proteases present in dentin and play an important role in the matrix collagen degradation. There are 11 CTs in humans . In dentin, has been described the CT-K (the most potent collagenase in mammalian), CT-L and CT-B . CTs form collagen active complexes with PG glycosaminoglycan (GAG) side chains, which can degrade collagen at multiple sites and generate multiple collagen fragments . It has been suggested there is synergistic activity between MMPs and CTs, as they are located very close together and near to the target substrate. The acidic activation of CTs may further activate dentin-bounded MMPs .
2.4. Strategies for the Stabilization of the Adhesive Interface
2.4.1. Nonselective MMPs Inhibitors
Within this group, the most commonly used substance is CHX, which efficiently inhibits the activity of MMPs for a short time even at low concentrations such as 0,2% [70, 71]. The effect of CHX is maintained for 18 months, at which time, the degradation of the adhesive interface begins. Although very little data have been published about the mechanism of action of CHX, this may be because chlorine behaves like an amphiphilic molecule that can bind to zinc of the catalytic domain of MMP, preventing its hydrolytic activity. Additionally, CHX is a cationic molecule that binds to the anionic molecules of both mineralized and demineralized dentin . The union of CHX with dentin is of the reversible electrostatic type and the activity time depends on the substantivity of CHX to treated dentin [9, 14, 71].
2.4.2. Biomodification of Dentin
Advances in tissue engineering have limited application in dental hard tissues due to their poor capacity to regenerate. This has led to the search for different strategies in which biomodification improves the physical properties of dentin by modifying their biochemistry.
(1) Physical Agents. The use of photo-oxidative techniques by the action of ultraviolet (UV) light requires the presence of an oxygen singlet, which is the most reactive and unstable type of the dioxygen molecule. Vitamin B2 (riboflavin) has been shown to be an important source of oxygen free radicals, including oxygen singlets. This vitamin, when activated by UV light, can induce the formation of covalent bonds mediated by oxygen singlets, between the amino group of glycine of a collagen chain, and the carbonyl groups of proline and hydroxyproline of side chains, leading to a cross-linking effect of collagen [24, 72, 73].
(2) Nonspecific Synthetic Agents of Collagen Cross-Linking. Cross-linking agents are substances that can bind to amino and carbonyl groups of the amino acid residues of the collagen, which stabilizes its structure and encompass it to make it more resistant to enzymatic degradation. Glutaraldehyde (GA) has great affinity for terminal amino groups, mainly the ɛ-amino groups of peptidyl-lysine and hydroxylysine residues of collagen . Less cytotoxic, carbodiimide (EDC) requires activation of the carboxylic groups of glutamic and aspartic acids to form an O-acyl isourea intermediate, which then reacts with the amino groups of lysine and hydroxylysine to form amino cross-linkages with collagen, with the release of urea. It has been reported that EDC requires a relatively long time (1 h) to cross-link the collagen, which limits its clinical use .
Although these substances have been shown to be effective in providing better stability of the adhesive interface , their biocompatibility has been questioned [24, 77]. Scheffel et al. (2015)  evaluated the cytotoxic effect of 5% GA and different concentrations of EDC on odontoblast-like cells with dentin barriers, and they concluded that 0,1; 0,3 and 0,5 M EDC and 5% GA did not induce transdentinal cytotoxic effect on odontoblast-like cells.
(3) Cross-Linking Agents of Natural Origin. These are antioxidant substances capable of promoting cross-linking with collagen and can inhibit the activity of MMPs. The cross-linking of the bioactive substances with collagen is nonenzymatic. Type I collagen provides tensile strength and cohesiveness properties  by endogenous covalent intermolecular cross-linking. The elastic strength-strain curve increases with an increasing degree of cross-linking .
The demineralized dentin has a significant decrease in its mechanical properties  and dentin biomodification improves mechanical properties through nonenzymatic collagen cross-linking , which can be attributed to the degree of cross-linking of the denuded collagen matrix.
It has been proposed that cross-linkers can inhibit the protease activity of MMPs and CTs by different mechanisms, such as down regulation of endogenous protease expression, protease inactivation/silencing and protection of cleavage sites within collagen modifying and hiding cleavage sites in the substrate , and avoiding the oxidation of cysteine switch. Within this group, anthocyanidins have been studied, mainly oligomeric proanthocyanidin. This is derived from grape seeds and improves the mechanical properties of previously demineralized dentin, such as tenacity and elastic modulus . Additionally, an increase in the contact angle of the water and a decrease in water vapor permeability has been demonstrated . However, the effects of these substances require very long application times (10 min to 1 h), a situation that does not make them clinically applicable . Furthermore, a reduction in the degree of conversion has been reported by inhibiting the polymerization of resin monomers  and brown pigmentation in dentin .
(4) Biomimetic Remineralization. The use of amorphous calcium phosphate nanoprecursors seeks to reproduce the natural biomineralization mechanisms of dentin [86, 87]. Although the incorporation of crystals in demineralized dentin has been achieved in vitro by means of lateral diffusion mechanisms, this process does not yet seem to be useful clinically .
2.4.3. Removal of Residual Water Not Bound to Collagen in the Hybrid Layer
Most methacrylates are hydrophobic and insoluble in water, which is why many manufacturers use ethanol as a solvent to ensure that they remain in solution in one phase. The application of these adhesives in water-saturated dentin after acid conditioning, generates separation in nanophases of adhesives . Pashley et al.  propose a change in the technique of wet adhesion where residual water is replaced by ethanol, which achieves a better penetration of the resin monomers in the collagen network and avoids the separation in nanophases of the adhesive, but they have an effect on partial inhibition of MMPs, less than alcohols with 4 methylene groups, which inhibit MMPs more effectively . The water molecule can be found attached to the collagen in a three-layer arrangement, or it can be found free. Ethanol can remove free water and half of the third layer of bound water , which decreases the separation between the collagen matrix and resin monomers and in turn, the possibility of action of collagenolytic enzymes.
Another approach to remove residual water is the use of SE primer adhesives with higher concentrations of functional molecules, such as 10-MDP (20-25 vol%), to which has been added only the water necessary to ionize the acidic monomers (20–25 vol%), which decreases the amount of water in the demineralization front . This dry technique proposes use of SE primer adhesives for 10 s, the conditioned dentin is dried and then sealed with a solvent-free adhesive, which produces a thin hybrid layer (1 μm) with good durability, but still prone to loss of bond strength over time [92, 93].
Dentin bonding is a challenge in clinical practice because it is a heterogeneous substrate with high protein content and is inherently humid. The presence of water in the adhesive interface constitutes a vehicle for the hydrolytic degradation of components of the hybrid layer. The stability of the dentin-resin interface is a necessary requirement for the durability of restorations; thus, different strategies have been proposed to control the different factors that result in its degradation.
Wet bonding techniques improve the immediate adhesive strength, and the use of dentin treatments with saturated alcohols, such as 100% ethanol, promotes the removal of water from the exposed collagen network to facilitate the penetration of adhesive monomers. However, this protocol requires a lot of clinical time and the durability of the restoration is compromised by not preventing the interface degradation.
Although CHX has been shown to have a beneficial effect on inhibiting the activity of MMPs in the adhesive interface, the duration of its effect for a limited time does not constitute a final solution to the problem of the degradation of the hybrid layer.
The biomodification of dentin is presented as an option that shows promising results. Cross-linking of the collagen in demineralized dentin improves the physical properties of dentin and makes it more resistant to degradation by the action of collagenolytic enzymes, in addition to the ability to inhibit the activity of MMPs and CTs by some cross-linking agents. However, all studies have been conducted in vitro since these substances have limitations that do not allow them to be used in a relevant clinical protocol. Due to this unresolved problem, it is necessary to continue with the search for new substances and techniques that can be used in a clinical protocol to improve the stability of the resin-dentin bonding interface, with which more durable adhesive restorations can be obtained.
Conflicts of Interest
The authors declare that they have no conflicts of interest.
- K. L. Van Landuyt, J. Snauwaert, J. De Munck et al., “Systematic review of the chemical composition of contemporary dental adhesives,” Biomaterials, vol. 28, no. 26, pp. 3757–3785, 2007.
- Y. Liu, L. Tjäderhane, L. Breschi et al., “Limitations in bonding to dentin and experimental strategies to prevent bond degradation,” Journal of Dental Research, vol. 90, no. 8, pp. 953–968, 2011.
- N. Nakabayashi, M. Nakamura, and N. Yasuda, “Hybrid Layer as a Dentin-Bonding Mechanism,” Journal of Esthetic and Restorative Dentistry, vol. 3, no. 4, pp. 133–138, 1991.
- D. H. Pashley, F. R. Tay, L. Breschi et al., “State of the art etch-and-rinse adhesives,” Dental Materials, vol. 27, no. 1, pp. 1–16, 2011.
- A. Mazzoni, P. Scaffa, M. Carrilho et al., “Effects of etch-and-rinse and self-etch adhesives on dentin MMP-2 and MMP-9,” Journal of Dental Research, vol. 92, no. 1, pp. 82–86, 2013.
- D. H. Pashley, F. R. Tay, C. Yiu et al., “Collagen degradation by host-derived enzymes during aging,” Journal of Dental Research, vol. 83, no. 3, pp. 216–221, 2004.
- Y. Nishitani, M. Yoshiyama, B. Wadgaonkar et al., “Activation of gelatinolytic/collagenolytic activity in dentin by self-etching adhesives,” European Journal of Oral Sciences, vol. 114, no. 2, pp. 160–166, 2006.
- M. R. O. Carrilho, R. M. Carvalho, M. F. de Goes et al., “Chlorhexidine preserves dentin bond in vitro,” Journal of Dental Research, vol. 86, no. 1, pp. 90–94, 2007.
- M. R. O. Carrilho, S. Geraldeli, F. Tay et al., “In vivo preservation of the hybrid layer by chlorhexidine,” Journal of Dental Research, vol. 86, no. 6, pp. 529–533, 2007.
- R. S. Blackburn, A. Harvey, L. L. Kettle, A. P. Manian, J. D. Payne, and S. J. Russell, “Sorption of chlorhexidine on cellulose: Mechanism of binding and molecular recognition,” The Journal of Physical Chemistry B, vol. 111, no. 30, pp. 8775–8784, 2007.
- J. De Munck, P. E. Van Den Steen, A. Mine et al., “Inhibition of enzymatic degradation of adhesive-dentin interfaces,” Journal of Dental Research, vol. 88, no. 12, pp. 1101–1106, 2009.
- L. Breschi, A. Mazzoni, F. Nato et al., “Chlorhexidine stabilizes the adhesive interface: a 2-year in vitro study,” Dental Materials, vol. 26, no. 4, pp. 320–325, 2010.
- V. Hass, I. V. Luque-Martinez, M. F. Gutierrez et al., “Collagen cross-linkers on dentin bonding: stability of the adhesive interfaces, degree of conversion of the adhesive, cytotoxicity and in situ MMP inhibition,” Dental Materials, vol. 32, no. 6, pp. 732–741, 2016.
- R. Seseogullari-Dirihan, F. Apollonio, A. Mazzoni et al., “Use of crosslinkers to inactivate dentin MMPs,” Dental Materials, vol. 32, no. 3, pp. 423–432, 2016.
- A. K. B. Bedran-Russo, P. N. R. Pereira, W. R. Duarte, J. L. Drummond, and M. Yamaychi, “Application of crosslinkers to dentin collagen enhances the ultimate tensile strength,” Journal of Biomedical Materials Research Part B: Applied Biomaterials, vol. 80, no. 1, pp. 268–272, 2007.
- S. Kermanshahi, J. P. Santerre, D. G. Cvitkovitch, and Y. Finer, “Biodegradation of resin-dentin interfaces increases bacterial microleakage,” Journal of Dental Research, vol. 89, no. 9, pp. 996–1001, 2010.
- A. Linde and M. Goldberg, “Dentinogenesis,” Critical Reviews in Oral Biology & Medicine, vol. 4, no. 5, pp. 679–728, 2016.
- L. Tjäderhane, M. R. Carrilho, L. Breschi, F. R. Tay, and D. H. Pashley, “Dentin basic structure and composition-an overview,” Endodontic Topics, vol. 20, no. 1, pp. 3–29, 2009.
- A. F. Montagner, M. P. M. Carvalho, and A. H. Susin, “Microshear bonding effectiveness of different dentin regions,” Indian Journal of Dental Research, vol. 26, no. 2, pp. 131–135, 2015.
- W. T. Butler, J. C. Brunn, and C. Qin, “Dentin extracellular matrix (ECM) proteins: comparison to bone ECM and contribution to dynamics of dentinogenesis,” Connective Tissue Research, vol. 44, no. 1, pp. 171–178, 2003.
- G. W. Marshall Jr., S. J. Marshall, J. H. Kinney, and M. Balooch, “The dentin substrate: structure and properties related to bonding,” Journal of Dentistry, vol. 25, no. 6, pp. 441–458, 1997.
- R. M. Carvalho, L. Tjäderhane, A. P. Manso, M. R. Carrilho, and C. A. Carvalho, “Dentin as a bonding substrate,” Endodontic Topics, vol. 21, no. 1, pp. 62–88, 2009.
- M. Saito and K. Marumo, “Collagen cross-links as a determinant of bone quality: a possible explanation for bone fragility in aging, osteoporosis, and diabetes mellitus,” Osteoporosis International, vol. 21, no. 2, pp. 195–214, 2010.
- A. K. Bedran-Russo, G. F. Pauli, S.-N. Chen et al., “Dentin biomodification: Strategies, renewable resources and clinical applications,” Dental Materials, vol. 30, no. 1, pp. 62–76, 2014.
- P. H. Dos Santos, S. Karol, and A. K. Bedran-Russo, “Long-term nano-mechanical properties of biomodified dentin-resin interface components,” Journal of Biomechanics, vol. 44, no. 9, pp. 1691–1694, 2011.
- G. Embery, R. Hall, R. Waddington, D. Septier, and M. Goldberg, “Proteoglycans in Dentinogenesis,” Critical Reviews in Oral Biology & Medicine, vol. 12, no. 4, pp. 331–349, 2016.
- K. A. Staines, V. E. MacRae, and C. Farquharson, “The importance of the SIBLING family of proteins on skeletal mineralisation and bone remodelling,” Journal of Endocrinology, vol. 214, no. 3, pp. 241–255, 2012.
- S. Suzuki, N. Haruyama, F. Nishimura, and A. B. Kulkarni, “Dentin sialophosphoprotein and dentin matrix protein-1: two highly phosphorylated proteins in mineralized tissues,” Archives of Oral Biolog, vol. 57, no. 9, pp. 1165–1175, 2012.
- P. A. Baldión, M. L. Velandia-Romero, and J. E. Castellanos, “Odontoblast-like cells differentiated from dental pulp stem cells retain their phenotype after subcultivation,” International Journal of Cell Biology, vol. 2018, Article ID 6853189, 12 pages, 2018.
- P. Bali, D. Kalaivanan, V. Divater, and . Logarani, “Matrix metalloproteinases: A double edge sword,” Dentistry and Medical Research, vol. 4, no. 1, pp. 3–8, 2016.
- S.-C. Zhang and M. Kern, “The role of host-derived dentinal matrix metalloproteinases in reducing dentin bonding of resin adhesives.,” International Journal of Oral Science, vol. 1, no. 4, pp. 163–176, 2009.
- M. Sulkala, T. Tervahartiala, T. Sorsa, M. Larmas, T. Salo, and L. Tjäderhane, “Matrix metalloproteinase-8 (MMP-8) is the major collagenase in human dentin,” Archives of Oral Biolog, vol. 52, no. 2, pp. 121–127, 2007.
- C. Chaussain, T. Boukpessi, M. Khaddam, L. Tjaderhane, A. George, and S. Menashi, “Dentin matrix degradation by host matrix metalloproteinases: Inhibition and clinical perspectives toward regeneration,” Frontiers in Physiology, vol. 4, pp. 1–8, 2013.
- L. Tjäderhane, H. Larjava, T. Sorsa, V.-J. Uitto, M. Larmas, and T. Salo, “The activation and function of host matrix metalloproteinases in dentin matrix breakdown in caries lesions,” Journal of Dental Research, vol. 77, no. 8, pp. 1622–1629, 1998.
- A. J. Smith, “Vitality of the dentinpulp complex in health and disease: growth factors as key mediators,” Journal of Dental Education, vol. 67, Article ID 678689, 2003.
- S. Fanchon, K. Bourd, D. Septier et al., “Involvement of matrix metalloproteinases in the onset of dentin mineralization,” European Journal of Oral Sciences, vol. 112, no. 2, pp. 171–176, 2004.
- M. Goldberg, A. B. Kulkarni, M. Young, and A. Boskey, “Dentin: structure, composition and mineralization,” Frontiers in Bioscience—Elite, vol. 3, no. 2, pp. 711–735, 2011.
- K. L. Van Landuyt, J. De Munck, J. Snauwaert et al., “Monomer-solvent phase separation in one-step self-etch adhesives,” Journal of Dental Research, vol. 84, no. 2, pp. 183–188, 2005.
- C. E. Brinckerhoff and L. M. Matrisian, “Matrix metalloproteinases: a tail of a frog that became a prince,” Nature Reviews Molecular Cell Biology, vol. 3, no. 3, pp. 207–214, 2002.
- S. Martin-De Las Heras, A. Valenzuela, and C. M. Overall, “The matrix metalloproteinase gelatinase A in human dentine,” Archives of Oral Biolog, vol. 45, no. 9, pp. 757–765, 2000.
- A. J. V. Strijp, D. C. Jansen, J. DeGroot, J. M. Ten Cate, and V. Everts, “Host-derived proteinases and degradation of dentine collagen in situ,” Caries Research, vol. 37, no. 1, pp. 58–65, 2003.
- C. Chaussain-Miller, F. Fioretti, M. Goldberg, and S. Menashi, “The role of matrix metalloproteinases (MMPs) in human caries,” Journal of Dental Research, vol. 85, no. 1, pp. 22–32, 2006.
- M. Sulkala, J. Wahlgren, M. Larmas et al., “The effects of MMP inhibitors on human salivary MMP activity and caries progression in rats,” Journal of Dental Research, vol. 80, no. 6, pp. 1545–1549, 2001.
- L. W. Boushell, M. Kaku, Y. Mochida, R. Bagnell, and M. Yamauchi, “Immunohistochemical localization of matrixmetalloproteinase-2 in human coronal dentin,” Archives of Oral Biolog, vol. 53, no. 2, pp. 109–116, 2008.
- T. Boukpessi, S. Menashi, L. Camoin, J. M. TenCate, M. Goldberg, and C. Chaussain-Miller, “The effect of stromelysin-1 (MMP-3) on non-collagenous extracellular matrix proteins of demineralized dentin and the adhesive properties of restorative resins,” Biomaterials, vol. 29, no. 33, pp. 4367–4373, 2008.
- Y. Shimada, S. Ichinose, A. Sadr, M. F. Burrow, and J. Tagami, “Localization of matrix metalloproteinases (MMPs-2, 8, 9 and 20) in normal and carious dentine,” Australian Dental Journal, vol. 54, no. 4, pp. 347–354, 2009.
- A. D. Loguercio, S. K. Moura, A. Pellizzaro et al., “Durability of enamel bonding using two-step self-etch systems on ground and unground enamel,” Operative Dentistry, vol. 33, no. 1, pp. 79–88, 2008.
- M. Hashimoto, H. Ohno, H. Sano et al., “Micromorphological changes in resin-dentin bonds after 1 year of water storage,” Journal of Biomedical Materials Research Part B: Applied Biomaterials, vol. 63, no. 3, pp. 306–311, 2002.
- M. Hashimoto, H. Ohno, H. Sano, M. Kaga, and H. Oguchi, “In vitro degradation of resin-dentin bonds analyzed by microtensile bond test, scanning and transmission electron microscopy,” Biomaterials, vol. 24, no. 21, pp. 3795–3803, 2003.
- J. Malacarne, R. M. Carvalho, M. F. de Goes et al., “Water sorption/solubility of dental adhesive resins,” Dental Materials, vol. 22, no. 10, pp. 973–980, 2006.
- M. Hashimoto, “A review—micromorphological evidence of degradation in resin-dentin bonds and potential preventional solutions,” Journal of Biomedical Materials Research Part B: Applied Biomaterials, vol. 92, no. 1, pp. 268–280, 2010.
- P. Spencer and Y. Wang, “Adhesive phase separation at the dentin interface under wet bonding conditions,” Journal of Biomedical Materials Research Part B: Applied Biomaterials, vol. 62, no. 3, pp. 447–456, 2002.
- Y. Wang, P. Spencer, X. Yao, and Q. Ye, “Effect of coinitiator and water on the photoreactivity and photopolymerization of HEMA/camphoquinone-based reactant mixtures,” Journal of Biomedical Materials Research Part A, vol. 78A, no. 4, pp. 721–728, 2006.
- J. Tanaka, K. Ishikawa, H. Yatani, A. Yamashita, and K. Suzuki, “Correlation of Dentin Bond Durability with Water Absorption of Bonding Layer,” Dental Materials, vol. 18, no. 1, pp. 11–18, 1999.
- B. Shokati, L. E. Tam, J. P. Santerre, and Y. Finer, “Effect of salivary esterase on the integrity and fracture toughness of the dentin-resin interface,” Journal of Biomedical Materials Research Part B: Applied Biomaterials, vol. 94, no. 1, pp. 230–237, 2010.
- E. L. Kostoryz, K. Dharmala, Q. Ye et al., “Enzymatic biodegradation of HEMA/bisGMA adhesives formulated with different water content,” Journal of Biomedical Materials Research Part B: Applied Biomaterials, vol. 88B, no. 2, pp. 394–401, 2009.
- N. Lehmann, R. Debret, A. Roméas et al., “Self-etching increases matrix metalloproteinase expression in the dentin-pulp complex,” Journal of Dental Research, vol. 88, no. 1, pp. 77–82, 2009.
- P. A. Baldion and C. J. Cortés, “Mathematical models of polymer-dentin physicochemical interactions and their biological effects,” Scientific Journal of Review, vol. 5, pp. 319–330, 2016.
- Y. K. Kim, L.-S. Gu, T. E. Bryan et al., “Mineralisation of reconstituted collagen using polyvinylphosphonic acid/polyacrylic acid templating matrix protein analogues in the presence of calcium, phosphate and hydroxyl ions,” Biomaterials, vol. 31, no. 25, pp. 6618–6627, 2010.
- S. E. Jee, J. Zhou, J. Tan et al., “Investigation of ethanol infiltration into demineralized dentin collagen fibrils using molecular dynamics simulations,” Acta Biomaterialia, vol. 36, pp. 175–185, 2016.
- L. E. Bertassoni, “Dentin on the nanoscale: Hierarchical organization, mechanical behavior and bioinspired engineering,” Dental Materials, vol. 33, no. 6, pp. 637–649, 2017.
- D. T. Fung, V. M. Wang, D. M. Laudier et al., “Subrupture tendon fatigue damage,” Journal of Orthopaedic Research, vol. 27, no. 2, pp. 264–273, 2009.
- F. R. Tay and D. H. Pashley, “Have dentin adhesives become too hydrophilic?” Journal of Canadian Dental Association, vol. 69, pp. 726–731, 2003.
- A. Mazzoni, D. H. Pashley, Y. Nishitani et al., “Reactivation of inactivated endogenous proteolytic activities in phosphoric acid-etched dentine by etch-and-rinse adhesives,” Biomaterials, vol. 27, no. 25, pp. 4470–4476, 2006.
- M. Iwasa, K. Tsubota, Y. Shimamura, S. Ando, M. Miyazaki, and J. A. Platt, “pH changes upon mixing of single-step self-etching adhesives with powdered dentin,” The Journal of Adhesive Dentistry, vol. 13, no. 3, pp. 207–212, 2011.
- C. Sabatini and D. H. Pashley, “Mechanisms regulating the degradation of dentin matrices by endogenous dentin proteases and their role in dental adhesion. A review,” American Journal of Dentistry, vol. 27, no. 4, pp. 203–214, 2014.
- V. Turk, V. Stoka, O. Vasiljeva et al., “Cysteine cathepsins: from structure, function and regulation to new frontiers,” Biochimica et Biophysica Acta—Proteins and Proteomics, vol. 1824, no. 1, pp. 68–88, 2012.
- S. Mahalaxmi, M. M. Madhubala, M. Jayaraman, and S. Sathyakumar, “Evaluation of matrix metalloproteinase and cysteine cathepsin activity in dentin hybrid layer by gelatin zymography,” Indian Journal of Dental Research, vol. 27, no. 6, pp. 652–656, 2016.
- P. M. C. Scaffa, L. Breschi, A. Mazzoni et al., “Co-distribution of cysteine cathepsins and matrix metalloproteases in human dentin,” Archives of Oral Biolog, vol. 74, pp. 101–107, 2017.
- R. Gendron, D. Grenier, T. Sorsa, and D. Mayrand, “Inhibition of the activities of matrix metalloproteinases 2, 8, and 9 by chlorhexidine,” Clinical and Diagnostic Laboratory Immunology, vol. 6, no. 3, pp. 437–439, 1999.
- M. R. Carrilho, R. M. Carvalho, E. N. Sousa et al., “Substantivity of chlorhexidine to human dentin,” Dental Materials, vol. 26, no. 8, pp. 779–785, 2010.
- A. Scott McCall, S. Kraft, H. F. Edelhauser et al., “Mechanisms of corneal tissue cross-linking in response to treatment with topical riboflavin and long-wavelength ultraviolet radiation (UVA),” Investigative Ophthalmology & Visual Science, vol. 51, no. 1, pp. 129–138, 2010.
- E. Choe and D. B. Min, “Chemistry and reactions of reactive oxygen species in foods,” Critical Reviews in Food Science and Nutrition, vol. 46, no. 1, pp. 1–22, 2006.
- A. Tezvergil-Mutluay, K. A. Agee, T. Uchiyama et al., “The inhibitory effects of quaternary ammonium methacrylates on soluble and matrix-bound MMPs,” Journal of Dental Research, vol. 90, no. 4, pp. 535–540, 2011.
- A. Tezvergil-Mutluay, K. A. Agee, T. Hoshika, F. R. Tay, and D. H. Pashley, “The inhibitory effect of polyvinylphosphonic acid on functional matrix metalloproteinase activities in human demineralized dentin,” Acta Biomaterialia, vol. 6, no. 10, pp. 4136–4142, 2010.
- A. Tezvergil-Mutluay, M. M. Mutluay, K. A. Agee et al., “Carbodiimide cross-linking inactivates soluble and matrix-bound MMPs, in vitro,” Journal of Dental Research, vol. 91, no. 2, pp. 192–196, 2012.
- A. Al-Ammar, J. L. Drummond, and A. K. Bedran-Russo, “The use of collagen cross-linking agents to enhance dentin bond strength,” Journal of Biomedical Materials Research Part B: Applied Biomaterials, vol. 91, no. 1, pp. 419–424, 2009.
- D. L. S. Scheffel, L. Bianchi, D. G. Soares et al., “Transdentinal cytotoxicity of carbodiimide (EDC) and glutaraldehyde on odontoblast-like cells,” Operative Dentistry, vol. 40, no. 1, pp. 44–54, 2015.
- M. Yamauchi and M. Shiiba, “Lysine hydroxylation and crosslinking of collagen.,” Methods in Molecular Biology (Clifton, N.J.), vol. 194, pp. 277–290, 2002.
- F. H. Silver, I. Horvath, and D. J. Foran, “Viscoelasticity of the vessel wall: the role of collagen and elastic fibers,” Critical Reviews in Biomedical Engineering, vol. 29, no. 3, pp. 279–301, 2001.
- Y. Liu, X. Bai, S. Li, Y. Liu, A. Keightley, and Y. Wang, “Molecular weight and galloylation affect grape seed extract constituents' ability to cross-link dentin collagen in clinically relevant time,” Dental Materials, vol. 31, no. 7, pp. 814–821, 2015.
- A. Jayakrishnan and S. R. Jameela, “Glutaraldehyde as a fixative in bioprostheses and drug delivery matrices,” Biomaterials, vol. 17, no. 5, pp. 471–484, 1996.
- R.-R. Liu, M. Fang, L. Zhang, C.-F. Tang, Q. Dou, and J.-H. Chen, “Anti-proteolytic capacity and bonding durability of proanthocyanidin-biomodified demineralized dentin matrix,” International Journal of Oral Science, vol. 6, no. 3, pp. 168–174, 2014.
- B. Green, X. Yao, A. Ganguly et al., “Grape seed proanthocyanidins increase collagen biodegradation resistance in the dentin/adhesive interface when included in an adhesive,” Journal of Dentistry, vol. 38, no. 11, pp. 908–915, 2010.
- A. Frassetto, L. Breschi, G. Turco et al., “Mechanisms of degradation of the hybrid layer in adhesive dentistry and therapeutic agents to improve bond durability - A literature review,” Dental Materials, vol. 32, no. 2, pp. e41–e53, 2016.
- F. R. Tay and D. H. Pashley, “Guided tissue remineralisation of partially demineralised human dentine,” Biomaterials, vol. 29, no. 8, pp. 1127–1137, 2008.
- L.-N. Niu, W. Zhang, D. H. Pashley et al., “Biomimetic remineralization of dentin,” Dental Materials, vol. 30, no. 1, pp. 77–96, 2014.
- T. Maravic, A. Mazzoni, A. Comba, N. Scotti, V. Checchi, and L. Breschi, “How Stable is Dentin As a Substrate for Bonding?” Current Oral Health Reports, vol. 4, no. 3, pp. 248–257, 2017.
- D. H. Pashley, F. R. Tay, R. M. Carvalho et al., “From dry bonding to water-wet bonding to ethanol-wet bonding. A review of the interactions between dentin matrix and solvated resins using a macromodel of the hybrid layer,” American Journal of Dentistry, vol. 20, no. 1, pp. 7–20, 2007.
- A. Tezvergil-Mutluay, K. A. Agee, T. Hoshika et al., “Inhibition of MMPs by alcohols,” Dental Materials, vol. 27, no. 9, pp. 926–933, 2011.
- N. Hiraishi, N. Nishiyama, K. Ikemura et al., “Water concentration in self-etching primers affects their aggressiveness and bonding efficacy to dentin,” Journal of Dental Research, vol. 84, no. 7, pp. 653–658, 2005.
- F. T. Sadek, C. S. Castellan, R. R. Braga et al., “One-year stability of resin-dentin bonds created with a hydrophobic ethanol-wet bonding technique,” Dental Materials, vol. 26, no. 4, pp. 380–386, 2010.
- L. Breschi, T. Maravic, S. R. Cunha et al., “Dentin bonding systems: From dentin collagen structure to bond preservation and clinical applications,” Dental Materials, vol. 34, no. 1, pp. 78–96, 2018.
Copyright © 2019 D. E. Betancourt et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.